Kaolinite
Laboratory syntheses

Syntheses of kaolinite at high temperatures (more than 100 °C) are relatively well known. There are for example the syntheses of Van Nieuwenberg and Pieters (1929); Noll (1934); Noll (1936); Norton (1939); Roy and Osborn (1954); Roy (1961); Hawkins and Roy (1962); Tomura et al. (1985); Satokawa et al. (1994) and Huertas et al. (1999). Relatively few low-temperature syntheses have become known (cf. Brindley and DeKimpe (1961); DeKimpe (1969); Bogatyrev et al. (1997)).

Laboratory syntheses of kaolinite at room temperature and atmospheric pressure have been described by DeKimpe et al. (1961). From those tests the role of periodicity becomes convincingly clear. DeKimpe et al. (1961) had used daily additions of alumina (as AlCl · 6 H O) and silica (in the form of ethyl silicate) during at least two months. In addition, adjustments of the pH took place every day by way of adding either hydrochloric acid or sodium hydroxide. Such daily additions of Si and Al to the solution in combination with the daily titrations with hydrochloric acid or sodium hydroxide during at least 60 days will have introduced the necessary element of periodicity. Only now the actual role of what has been described as the "aging" (Alterung) of amorphous alumino-silicates (as for example Harder, 1978 had noted) can be fully understood. As such, time is not bringing about any change in a closed system at equilibrium; but a series of alternations of periodically changing conditions (by definition, taking place in an open system) will bring about the low-temperature formation of more and more of the stable phase kaolinite instead of (ill-defined) amorphous alumino-silicates.
punctuation:no_comma